Determination of Early Age Mortar and Concrete Strength by ... of Early Age Mortar and Concrete...
Embed Size (px)
Transcript of Determination of Early Age Mortar and Concrete Strength by ... of Early Age Mortar and Concrete...
Determination of Early Age Mortar and Concrete Strength by Ultrasonic Wave Reflections
Thomas Voigt1, Yilmaz Akkaya2, Surendra P. Shah3
Keywords: nondestructive tests, ultrasonic tests, compressive strength, concrete, mortars, hydration, wave reflection, transverse waves
The in-situ testing of early age concrete strength is crucial for determining the time of form removal from concrete elements, opening highways to traffic or applying of prestress to steel reinforcement. A nondestructive ultrasonic technique, which measures the reflection loss of ultrasonic transverse waves at a concrete-steel interface, is presented in this paper. The focus is to compare wave reflection measurements on mortar and concrete to strength. It is shown that the reflection loss is linearly related to the strength gain of mortar and concrete at early ages. The experiments have revealed a relationship between the homogeneity of the tested materials and the consistency of the reflection measurements. The repetition of simultaneous measurements of wave reflections and compressive strength on mortar results in similar strength-reflection loss relationships. Multiple measurements on the same concrete gave multiple strength-reflection loss relationships. The accuracy of the strength predictions made with the proposed method is discussed and compared to other nondestructive test methods. 1 Dipl.-Ing., Research Associate, Center for Advanced Cement-Based Materials, Northwestern University, 2145 Sheridan Road, Evanston, Illinois 60208. Email: firstname.lastname@example.org, Corresponding Author 2 Ph.D., Research Associate, Center for Advanced Cement-Based Materials, Northwestern University, 2145 Sheridan Road, Evanston, Illinois 60208. Currently at Istanbul Technical University, Civil Engineering Faculty, Maslak, 80626, Istanbul, Turkey. Email: email@example.com 3 Prof. for Civil Engineering, Director of Center for Advanced Cement-Based Materials, Northwestern University, 2145 Sheridan Road, Evanston, Illinois 60208. Email: firstname.lastname@example.org.
The technological progress of the last decade has brought a tremendous change to many fields of the civil engineering sciences. A representative indicator is the development of numerous sophisticated techniques for nondestructive testing of cementitious materials. The great variety of methods is based on acoustical, electrical, magnetic, mechanical, optical, radiographic, and thermal properties of the tested materials. This paper reports on a wave reflection method based on ultrasonic wave propagation. In the following, a short overview is given about the development of the method and various applications of this technique that can be found in the literature.
Papadakis (1968) described experiments with a buffer rod bonded to a sample material. A transducer at the free end of the buffer rod was used to generate ultrasonic waves and to monitor the reflections from the buffer-sample interface and from the far end of the sample. From the amplitude ratios of certain echoes the reflection coefficient at the interface and the ultrasonic attenuation in the sample were calculated.
The first application of the method to cementitious materials was reported by Stepinik et al. (1981). The reflections of transverse waves (T-waves) at the interface between a quartz bar and cement paste were monitored and used to calculate the reflection coefficient at the interface as well as the shear modulus and dynamic viscosity of the cement paste. The measured quantities were found to be sensitive indicators of the hydration process at early ages. Based on these experiments Vali and Stepinik (1998, 1999) have investigated the hydration of gypsum, various types of cement pastes and epoxy. In another study Vali (2000) investigated the hydration of cement paste as it is affected by different admixtures. The measurement of the reflection coefficient could reflect the various hydration kinetics.
ztrk et al. (1999) adapted the wave reflection technique to concrete. The reflection coefficient was calculated from T-wave reflections at the interface between the concrete and a steel plate. The values of the reflection coefficient of concretes containing different admixtures were correlated to pin penetration tests and concrete temperature measurements. A distinct point in the development of the reflection coefficient was found to be related to the initial setting time and the end of the induction period in the hydration process. In continuation of this work Rapoport et al. (2000) advanced this theory further and additionally compared the development of the shear moduli determined by wave reflection measurements and the vibrational resonance frequency method. The wave reflection method as described in these papers has a high potential for further field applications.
A combined study of the hydration process of cement paste is reported by Chotard et al. (2001). The experimental setup is similar to that introduced by Papadakis (1968). The reflection coefficient and the longitudinal wave (L-wave) velocity was compared to results from shrinkage measurements, X-ray diffraction, differential thermal analysis and thermogravimetric measurements. The ultrasonic parameters proved to be sensitive to the formation and structuring of hydration products.
In a recent study by Akkaya et al. (2002) the wave reflection method was used to monitor the strength development of concrete. The compressive strength was found to be linearly related to the wave reflection measurements performed under isothermal and outdoor conditions and a
procedure for the strength prediction was developed. The experiments have shown that the method can reliably assess the early-age strength gain of concrete.
PHYSICAL INTERPRETATION OF THE REFLECTION COEFFICIENT
The wave reflection method monitors the development of the reflection coefficient at the interface between two materials over time. When a longitudinal or transverse wave is reflected at a boundary between Material 1 and Material 2 the reflection coefficient r can be calculated as
where 1 and 2 are the density of the Materials 1 and 2 and v1 and v2 the wave velocity in the Materials 1 and 2 respectively. Knowing the density and the T-wave velocity vT of a material the dynamic shear modulus can be calculated as follows:
2TvG = . (2)
The interconnection of r and G expressed by Equations 1 and 2 shows that the reflection coefficient measured with transverse waves can theoretically be related to dynamic shear modulus G. Consequently, the reflection coefficient determined with transverse waves is governed by the development of the dynamic shear modulus. The development of shear modulus as a mechanical property of the material is related to how the microstructure of hydrating cement evolves as a result of curing. The compressive strength of cementitious materials also depends on the progress of the cement hydration. Accordingly, with reflection coefficient and compressive strength, two parameters with a direct physical relationship to the evolving properties of the test material are compared.
EXPERIMENTAL PROCEDURE AND APPARATUS
The experiments described in this paper are based on wave reflection measurements at an interface between a buffer material and a cementitious test material (e.g. concrete). For all experiments the wall or bottom plate of a steel mold (wall thickness = 12 mm) was used as the buffer material. The dimensions of the mold are 10x8x41 cm. A transducer with a center frequency of 2.25 MHz transmits a T-wave pulse into the steel. When the wave encounters the steel-concrete interface, part of the wave energy is transmitted into the concrete and part is reflected back to the transducer. Some of this wave energy is then again reflected from the transducer-steel interface into the steel and is again partially reflected when it hits the steel-concrete boundary. The described process is shown in Fig. 1, where ST is the Transducer signal transmitted into the steel, R1 and R2 are the first and second reflection captured by the transducer and T1 and T2 are the first and second transmission into the concrete.
The measurements start directly after placing the fresh concrete. When the concrete is liquid, the entire wave energy, which is approaching the interface, is reflected, since T-waves cannot propagate in liquids. Thus, the reflection coefficient is unity. With proceeding hydration
the cement grains percolate and build up a skeleton allowing the T-waves to propagate. With increasing hydration time the ability of the concrete to transmit T-waves gains higher levels. More and more wave energy is transmitted into the concrete and the reflection coefficient decreases rapidly. After a certain time this process slows down and the reflection coefficient approaches a final value. At this time changes in the microstructure of the concrete due to hydration are too small to alter the T-wave propagation properties significantly.
The reflections R1 and R2 are acquired in time domain (Fig. 2(a)) and then transformed into frequency domain using a fast Fourier transform (FFT) algorithm (Fig. 2(b)). The separation of the reflections in time domain for the given steel plate thickness is about 7 s. The reflection factor is calculated from the first and second reflections represented in frequency domain. The following procedure is applied to isolate the reflection coefficient. The first reflection can be written as
( ) 21T1 drdSfF = (3)
where F1(f) is the FFT of the first reflection in terms of the frequency f; ST the transducer function inclu